The FactOptimal Module FactOptimal is programmed to identify the optimal conditions for alloy and process design using thermodynamic and property databases, FactSage software and the Mesh Adaptive Direct Search Algorithm. A.Gheribi, E. Bélisle, C.W. Bale and A.D. Pelton CRCT, Ecole Polytechnique de Montréal S. Le Digabel and C. Audet, GERAD, Ecole Polytechnique de Montréal Table of contents Section Section Section Section Section Section Section Section Section Section Section Section Section 1 2 3 4 5 6 7 8 Introduction How does FactOptimal Work – Using the stored examples Example 1 : Maximize an adiabatic flame temperature Example 2 : Calculation of minimum liquidus temperature under constraints Example 3 : How to use equality constraints Example 4 : FactOptimal coupled with solidification software Introduction to the Pareto concept Example 5 : Optimize 2 properties with two files (linked) Pgas vs density (T2 = T1+20) 9 Example 6 : Application using the cache option (Next Run) 10 Example 7 : Target optimization 11 Optimization using the Function Builder 12 Example 8 : Calculation of characteristic points on the liquidus surface 13 Characteristic points – reciprocal systems www.factsage.com The FactOptimal Module Table of contents (cont.) Section Section Section Section Section Section 14 Example 9 : Characteristic points – closest characteristic point 15 Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE 16 Example 11 : Improvement of the mechanical properties of 7178 aluminum alloy 17 Example 12 : Improve the texture and grain refinement properties at low temperature 18 Example 13 : Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus 19 Example 14: Double target optimization www.factsage.com Introduction - 1 - The Equilib module can be used to screen potential systems, searching for compositions having a desired set of properties and phase constitution, under a given set of constraints - For instance, one could search for alloys within a given composition range, with a liquidus temperature below xoC, with a desired freezing range, with a maximum or minimum amount of precipates after annealing at yoC, with a density or shrinkage ratio within a given range, etc. One could also search for optimal annealing or rolling temperatures, for example. - However, to perform such searches “by hand” for a multicomponent alloy by simply performing thousands of calculations over a grid of compositions is extremely time-consuming. - FactOptimal extends the capability of Equilib by coupling it with a Mesh Adaptive Direct Search method algorithm (MADS) developed at GERAD by S. Le Digabel and C. Audet, Ecole Polytechnique de Montreal FactOptimal 1.1 www.factsage.com The FactOptimal Module What’s New In FactOptimal 6.4 ? Double Target calculations: one can now target two properties simultaneously. Continue run after a target calculation: it is now possible to click on “continue run” to calculate another composition corresponding to the desired target. Additional properties for optimization or constraints : physical properties (density, thermal expansion, viscosity, thermal conductivity, electrical conductivity…) are now available. For cooling calculations, the annealing temperature can now be chosen as an optimizable variable. Logarithmic values: one can optimize the logarithm of a property e.g log(activity) or log(P). In certain cases this may present a numerical advantage, increasing speed and precision. When using two input files, the "linked" button previously allowed using the temperature from the first file as a variable for the second file. In FactOptimal 6.4, amount of reactants and pressure can also be used. A function saved with Function Builder can now be used as a property constraint. When characteristic points on a liquidus surface are calculated, the results are now shown in a table as well as on a graph, displaying detailed compositions, temperature and the solid phases in equilibrium with the liquid. FactOptimal 1.2 www.factsage.com The FactOptimal Module What’s New In FactOptimal 6.4 ? (cont.) There is now an option to calculate the minimum or maximum on a liquidus surface closest to the initial composition. When calculating characteristic points on a liquidus surface, there is a new option either to calculate the lowest minimum first or to calculate all minima with no priority. There is a new parameter to limit the maximum time for the optimization. When working with variables of type “real”, a new parameter is available: the decimal precision. Results displayed in a table (target type calculations or characteristic points on a liquidus. surface) can now be saved as an Excel file. When using two input files, property constraints can now be applied on either file. When no feasible solution is found, FactOptimal now displays the closest solution (example on page 4.20). FactOptimal 1.3 www.factsage.com The FactOptimal Module What was New In FactOptimal 6.3 ? Target calculations : in addition to minimizing/maximizing one can now target a specific value. Additional new property for optimization : activity of a phase/species. Additional new variables : temperature and pressure. Additional new property constraint : activity of a phase/species. The sum of composition variables can now be greater than 1. Thus, variables can now be of type integer or real. When using two input files, the "linked" button is now activated in order to use the temperature from the first file in the second file. When using two input files, properties constraints can now apply to each of the input files. Latest optimizations are saved with Equilib files and can be recalled by using the “Recent” button Convenient MIN/MAX buttons to set all minimum/maximum values of composition variables For a Scheil cooling system, the mass of specific species/phase(s) can now be optimized Better optimization for composition constraints having equality rules Table display of result for the special points option Use of cache file to restart any optimization from the latest calculation FactOptimal 1.4 www.factsage.com General recommendations In general, we recommend that you perform every optimization twice, using different starting points. If you are not sure of the best starting point, a good practice is to use the Q-Random option. See p. 3.8 and p. 19.5 for detailed examples. Do not hesitate to use the « Continue Run >> » option to make sure there is no better answer when you have completed the maximum number of calculations entered in the parameters (see example 6). If you need more information or if you have specific questions about FactOptimal, please contact Aimen Gheribi ([email protected]) or Eve Bélisle ([email protected]). FactOptimal 1.5 www.factsage.com Introduction - 2 ◦ The purpose of FactOptimal is to minimize and/or maximize a set of functions: {f1(x1,x2..T, P); f2(x1,x2….T, P)} ◦ The functions are calculated by Equilib ◦ The functions may be non-smooth (e.g. liquidus ) ◦ The estimation of derivatives is problematic ◦ Evaluations of f can be time consuming ◦ The function calculation may fail unexpectedly at some points ◦ The constraints may be non-linear, non-smooth or Boolean FactOptimal 1.6 www.factsage.com How does FactOptimal work ? – 1 Equilib Text file NOMAD (Nonsmooth Optimization by Mesh Adaptive Direct Search) In memory XML FactOptimal Commands . macro processing Calculator (bb.dll) XML FactOptimal 2.1 www.factsage.com How does FactOptimal work ? – 2 The principal of the optimization is a loop where FactOptimal sends compositions to Equilib, then Equilib returns the values of the properties to be optimized to FactOptimal. This is repeated until the properties minimum or maximum of is reached. For example, the minimization of the liquidus temperature of the KCl-RbCl-CsCl salt system can be represented by : FactOptimal 2.2 www.factsage.com Using the stored examples The following examples are stored on your computer. In Equilib click on ‘File > Open > Directory > Fact Optimal Examples’ > Fact Optimal 1 (Maximum adiabatic ...’). In the Menu Window click on ‘Calculate ’ and then in the Results Window click the FactOptimal icon. In the Fact Optimal Window click on ‘Recent ...’to load the stored example. FactOptimal 2.3 www.factsage.com Examples of FactOptimal www.factsage.com Example 1: Maximize an adiabatic flame temperature - 1 The objective is to maximize the adiabatic flame temperature of : (1-A) CH4 + (A) O2 By varying A from 0 to 1 in steps of 0.01, you can calculate the adiabatic flame temperature as a function of A using the Equilib module (see Equilib regular slide show, section 10). Plotting the results you find that: Tad ,max ~3075 K when A ~0.65 FactOptimal 3.1 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 2 To calculate the maximum temperature with FactOptimal, the first step is to perform a single equilibrium calculation at any arbitrary composition and then open FactOptimal. FactOptimal Icon FactOptimal 3.2 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 3 When you “click” on the FactOptimal icon the first window of the module appears. If you are using the stored example files, click on “Recent...” to load the FactOptimal file. There are 5 tabs. The first tab is “Properties” where we define the quantities to minimize and/or maximize. In this example, we specify that : 1 - we consider one property 2 - we want to maximize this property 3 - the property is temperature 1 2 3 Click on Next to go to the Variables tab FactOptimal 3.3 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 4 In the “Variables” tab we define the permissible range of composition and the initial values for the first estimate. Alternatively, select “Q-Random” and let the program choose the initial values. (see page 3.8) Use “ALL” buttons to set the same value for all variables. REAL type is chosen with values varying from 0 to 1. For INTEGER type, see example in section 3.7. Only composition variables are used in this example. Click on Next to go to the Constraints tab. FactOptimal 3.4 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 5 In the “Constraints” tab the sum of composition variables is set by default to 1. In the “Parameters” tab we define the maximum number of Equilib calculations and the search region. If the initial point is a good estimate of the expected answer, choose Small (0.1), otherwise choose Large (1) or Medium (0.5). The program will stop after the selected maximum number of Equilib calculations, or it may converge earlier. The number of calculations can be extended later if desired without losing the first set of calculations. Similarly, the stop button can be used at any time to terminate the optimization calculations. See section 9 for more details. Click on the “Calculate >>” button to start the optimization. FactOptimal 3.5 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 6 We obtain the results after 25 Equilib Calculations. The Equilib Results Window with the equilibrium calculation corresponds to the calculated maximum adiabatic flame temperature. FactOptimal 3.6 www.factsage.com Example 1: Maximize an adiabatic flame temperature - 7 To decrease the number of significant digits and thereby decrease the computation time, you can choose to work with INTEGER type variables. FactOptimal 3.7 Using the same example, INTEGER type is chosen with values varying from 0 to 1000. By selecting this option as opposed to real values varying from 0 to 1, we are limiting the number of significant digits to 3. www.factsage.com Example 1: Maximize an adiabatic flame temperature - 8 We also clicked the Q-Random (Quasi-Random) option, in order to let FactOptimal determine the best initial point. This is a good practice if you are not sure of what the best starting point should be. When choosing this option, we have to define the number of such calculations. In the present example 50 quasi-random calculations will be performed in order to get the best initial point, then 25 subsequent Equilib calculations will be performed to determine the best solution for a total of 75 calculations. FactOptimal 3.8 www.factsage.com Example 2: Minimize the liquidus temperature under constraints In this section we will calculate the minimum liquidus temperature of a multicomponent solution phase under various constraints of composition, cost, density, etc. There are 2 examples – • • minimize the liquidus temperature of an Al-Cu-Mg-Zn molten alloy using data from FTlite minimize the liquidus temperature of a LiCl-NaCl-KCl-LiF-NaF-KF molten salt using data from FTsalt www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 1 System: Al-Cu-Mg-Zn. Constraints: • Sum of mole fractions (XAl + XCu) < 0.2 • Density < 2.2 g/ml • Cost < 2900 $/ton Step 1: Using Equilib define the system and select the appropriate database: FTlite. FactOptimal 4.1 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 2 Step 2: Perform a single equilibrium calculation at an arbitrary composition and specify a precipitate (P) calculation on the liquid (i.e. liquidus temperature calculation) and “include molar volumes” (for the calculation of the density): FactOptimal 4.2 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 3 Equilib Results Window Click on the FactOptimal icon FactOptimal 4.3 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 4 Step 3: Click on the FactOptimal icon and set up the calculation. If you are using the stored example files, click on “Recent...” to load the Fact Optimal file. In this example, we specify that: 1. we consider one property 2. we want to minimize this property 3. the property is Temperature 1 2 4. the Cost is to be included in the optimization 3 4 FactOptimal 4.4 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 5 Step 4: In the "Variables" tab we define the permissible composition range (and initial estimates) 0.05 ≤ Wt.% Al ≤ 0.2 0.05 ≤ Wt.% Cu ≤ 0.2 0.75 ≤ Wt.% Mg ≤ 0.9 0.00 ≤ Wt.% Zn ≤ 0.15 FactOptimal 4.5 (0.05) (0.02) (0.75) (0.03) www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 6 Step 5: In the "cost" tab we define the unit price of each component. The cost per unit can be in $/ton, $/kg or $/g $2132 per ton Al $7315 per ton Cu $2980 per ton Mg $2100 per ton Zn FactOptimal 4.6 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 7 Step 6: Define the constraints on composition: X(Al) + X(Cu) < 0.2 SUM (Comp. Variables) = 1 therefore compositions are mole fractions FactOptimal 4.7 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 8 Step 7: Define the constraints on properties : r < 2.2 g/ml cost < 2900 $/Ton FactOptimal 4.8 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 9 Step 8: Enter the maximum number of Equilib calculations and the initial search region (see slide 3.5). The max number of calculations is 150 because previous calculations have shown this number is necessary to obtain convergence. FactOptimal 4.9 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 10 FactOptimal Results Window Save and print the graph or change the axis scale Minimum Composition at the minimum Values of the defined constraints: X(Al) + X(Cu) < 0.2 r < 2.2 g/ml cost < 2900 $/Ton FactOptimal 4.10 www.factsage.com Example 2a : Minimize the alloy liquidus temperature under constraints - 11 Equilib Results Window FactOptimal 4.11 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 1 This is a typical problem to solve for the design of a molten salt medium for thermal storage System: LiCl-NaCl-KCl-LiF-NaF-KF Constraints: • • • • • wt.%(LiCl) + wt.%(LiF) ≤ 10 wt.%(NaCl) + wt.%(KCl) ≥ 3*(wt.%(NaF) + wt.%(KF)) Density ≥ 1750 kg/m3 Cp ≥ 1250 J/kg Cost ≤ 3.5 $/kg Step 1: Using Equilib, define the system and select the appropriate database: FTsalt. Use a basis of 1000g FactOptimal 4.12 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 2 Step 2: Perform a single equilibrium calculation at an arbitrary composition and specify a precipitate (P) calculation on the liquid (i.e. liquidus temperature calculation) and “include molar volumes” (for the calculation of the density): FactOptimal 4.13 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 4 Step 3: After doing one calculation, click on the FactOptimal icon and set up the optimization. If you are using the stored example files, click on “Recent...” to load the Fact Optimal file. In this example, we specify that: 1. we consider one property 2. we want to minimize this property 3. the property is Temperature 1 2 4. the Cost is to be included in the optimization 3 4 FactOptimal 4.14 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 5 Step 4: Define the permissible composition range and a set of initial estimates. Here we are not sure of the best starting point so we used the Q-Random option. FactOptimal 4.15 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 6 Step 5: In the "cost" tab we define the unit price of each component. FactOptimal 4.16 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 7 Step 5: Define the constraints on composition. • • • Sum (Comp. Variables) = 1000 g wt.%(LiCl) + wt.%(LiF) ≤ 10 wt.%(NaCl) + wt.%(KCl) ≥ 3*(wt.%(NaF) + wt.%(KF)) FactOptimal 4.17 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 8 Step 6: Define the constraints on properties. • • • FactOptimal 4.18 Density ≥ 1750 kg/m3 Cp ≥ 1250 J/kg Cost ≤ 3.5 $/kg www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 9 Step 7: Enter the maximum number of Equilib calculations and the initial search region (see slide 3.5). Here we tried 500 calculations with 500 Quasoi-Random calcuations for a total of 1000 calculations. We used a large search region. FactOptimal 4.19 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 10 FactOptimal Results Window: Unfortunately, after 1000 calculations, FactOptimal did not find any answer respecting the constraints. Here the closest results are shown in a table. FactOptimal 4.20 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 11 Here we change constraints on composition and cost. The new constraints are : wt.%(LiCl) + wt.%(LiF) ≤ 100 wt.%(NaCl) + wt.%(KCl) ≥ (NaF + KF) Density ≥ 1750 kg/m3 Cp ≥ 1250 J/kg Cost ≤ 5.5 $/kg FactOptimal 4.21 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 12 FactOptimal Results Window: with the new set of constraints, FactOptimal finds the lowest liquidus temperature to be 577.39ºC. FactOptimal 4.22 www.factsage.com Example 2b: Minimize the salt liquidus temperature under constraints - 13 Equilib Results Window FactOptimal 4.23 www.factsage.com Example 3 : How to use equality constraints - 1 Using the example from section 3, we will calculate the maximum adiabatic flame temperature when O2 is replaced by air where moles O2 = moles N2/4. FactOptimal 5.1 www.factsage.com Example 3 : How to use equality constraints - 2 We want the following constraints to be respected (molar basis): CH4 + O2 + N2 = 1 O2 = N2/4 To enter these constraints in FactOptimal, they must be converted to allow only one degree of freedom : O2 = -1/5*CH4 + 1/5 N2 = -4/5*CH4 + 4/5 That is, if there are m composition variables (C1, C2, ... Cm) and n equations relating these variables, then the first (m-n) variables must be expressed as functions of the remaining variables as Ci = f(Cm-n+1,...Cm); i ≤ (m-n) FactOptimal 5.2 www.factsage.com Example 3 : How to use equality constraints - 3 The SUM (Comp. variables) option must always be unchecked when equality constraints are being used. FactOptimal 5.3 www.factsage.com Example 3 : How to use equality constraints - 4 The adiabatic flame temperature in air is less than in O2. FactOptimal 5.4 www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 1 System: Al-Ce-Mg-Zn Step 1: Using Equilib we define the system and select the appropriate databases FTlite. The arbitrary composition corresponds to approximately the composition of AZ31 alloys. FactOptimal 6.1 www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 2 Step 2: Perform a single Equilib calculation using the solidification software and choosing a Scheil-Gulliver Cooling type calculation (see Equilib Advanced Slide Show, slide 13.1) FactOptimal 6.2 www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 3 Step 3: Click on the FactOptimal icon and set up the calculation. If you are using the stored example files, click on “Recent...” to load the Fact Optimal file. In this example, we specify that : 1. we consider one property 2. we want to maximize this property 3. the property that we consider is the total mass of precipitates after a subsequent annealing Click on the Annealing box to activate the “mass of precipitate” option. The Anealing selection menu will pop-up FactOptimal 6.3 www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 4 Step 4: Select the Annealing phase in the annealing selection window. Here we choose the primary phase (HCP) and define the annealing temperature (500 oC). Select the phase that is the matrix for the precipitation calculation. This is the equivalent of double clicking on the amount in the Summary Page of the Equilib Results Window. FactOptimal 6.4 www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 5 The Mass fraction of precipitates option can now be selected In the variables tab, define the permissible composition ranges: 96.5 > Wt.% Mg > 92.5 2 > Wt.% Ce 3.5 > Wt.% Al > 2.5 1 > Wt.% Zn > 2 FactOptimal 6.5 In the “Constraints” tab : - Sum(Comp. variables) = 100 (output desired as wt.%) In the “Parameters” tab : - 150 Equilib calculations - initial search region “large” (i.e. 1) www.factsage.com Example 4 : Maximize the total mass of all precipitates in the hcp matrix for an (AZ31+Ce) Mgbased alloy after Scheil-Gulliver cooling and subsequent full annealing - 6 FactOptimal Results Window Total elapsed time You can use the zoom icon to change the axis limits. FactOptimal 6.6 www.factsage.com The Pareto Concept - the simultaneous minimum and/or maximum of more than one function. Pareto front All other points Example of a Pareto Front. 1.0 0.8 0 < P2 < 1 C 0.6 A B 0.4 0.2 P1(C)>P1(A) P2(C)>P2(B) 0.0 0.0 0.2 0.4 0.6 0 < P1 < 1 0.8 1.0 We want to simultaneously minimize properties P1 and P2. All points shown are calculated. Blue points are on the Pareto front. For any point not on the Pareto Front (for example point C), “better” points can be found on the Pareto front. That is, for the same value of P1 as at point C there is a point on the Pareto front with a lower value of P2, and for the same value of P2 as at point C there is a point on the Pareto front with a lower value of P1. You must then select the optimal composition on the Pareto Front according to your requirements. FactOptimal 7.1 www.factsage.com Example 5 : Minimize the density and maximize Cp under constraints on Tliq - 1 This example calculates a Pareto Front. System: Properties: LiCl-NaCl-KCl-CaCl2-MgCl2 Maximize density at Tliq and minimize the heat capacity at (Tliq + 20ºC). Constraints: Liquidus temperature Tliq below 610 oC . Step 1: Define the system and select the appropriate database FTSalt. Two separate Equilib calculations are required, the first to calculate the liquidus temperature and density, and the 2nd to calculate Cp. - First file (this is the active file): Select a precipitate target (P) on the liquid and click “include molar volumes” so as to calculate density - Second file (this is a stored file that will be used later in the calculation): A normal calculation (without the P option) at an arbitrary temperature Press Calculate FactOptimal 8.1 www.factsage.com Example 5 : Minimize the density and maximize Cp under constraints on Tliq - 2 First file - Calculate and click the FactOptimal icon. If you are using the stored example files, click on “Recent...” to load the Fact Optimal file. In this example, we specify that : 1- we consider two properties, density and Cp 2- we want to maximize the first property and minimize the second 3 – we want to link the second property defined in the stored file For the 2nd property, the calculation is performed using the precipitate (liquidus) temperature and adding 20ºC, using the stored second file. Enter the location of the second file here. (Use browse) FactOptimal 8.2 www.factsage.com Example 5 : Minimize the density and maximize Cp under constraints on Tliq - 3 Define the constraints on properties: Tliq < 610 oC FactOptimal 8.3 www.factsage.com Example 5 : Minimize the density and maximize Cp under constraints on Tliq - 4 Set up the parameters: FactOptimal 8.4 www.factsage.com Example 5 : Minimize the density and maximize Cp under constraints on Tliq - 5 FactOptimal Results Window One can perform an Equilib calculation at any point on the Pareto Front by clicking on it in the graph and and opening it in the Equilib module. The compositions on the Pareto Front can be saved and opened in Text, Excel,...... One can re-plot all calculated points or show only the Pareto front. FactOptimal 8.5 www.factsage.com Example 6 : Application using the cache option (Next Run) - 1 In some cases you may wish to stop a calculation before the convergence criterion has been met, or before the specified number of Equilib calculations has been reached. Alternatively, Equilib may fail to converge, especially for complex calculations. The cache option permits you to restart the optimization procedure and carry on from the last calculation. In this example we use the FTSalt database with 8 reactants. FactOptimal 9.1 www.factsage.com Example 6 : Application using the cache option (Next Run) - 2 An Equilib calculation is first made at an arbitrary composition and temperature. FactOptimal 9.2 www.factsage.com Example 6 : Application using the cache option (Next Run) - 3 The objective is to optimize both composition and temperature in order to maximize the amount CaFCl (solid) at equilibrium. FactOptimal 9.3 www.factsage.com Example 6 : Application using the cache option (Next Run) - 4 Each input constituent can vary between 0 and 1000 moles. We choose the INTEGER type of variable in order to reduce the precision and thus decrease the time to convergence. We allow the temperaure to vary between 300K and 1000K every +/-1 degree (precision). Note that the temperature variable is of the INTEGER type. FactOptimal 9.4 www.factsage.com Example 6 : Application using the cache option (Next Run) - 5 The maximum number of Equilib calculations is set to 2000. FactOptimal 9.5 www.factsage.com Example 6 : Application using the cache option (Next Run) - 6 We stop the calculation after 166 calculations, at which point FactOptimal has obtained a value of 456 mol of CaFCl at 557K. Click on the ‘Continue Run’ button to continue the optimization from the last point, using the previously saved calculations (cached). FactOptimal 9.6 www.factsage.com Example 6 : Application using the cache option (Next Run) - 7 Next we stop the calculation after an additional 253 calculations, at which point FactOptimal has found a better value of 465 moles at 336K. FactOptimal 9.7 www.factsage.com Example 6 : Application using the cache option (Next Run) - 8 Next run FactOptimal for 345 more calculations, at which point FactOptimal has found a better value of 494 moles at 325K. FactOptimal 9.8 www.factsage.com Example 7 : Target Optimization - 1 Using the same system as Example 3 (slide 6.1) (LiCl-NaCl-KCl-CaCl2-MgCl2) let us perform a target calculation whereby we search for compositions where the density of the liquid at the liquidus temperature is 2.00 g/ml. FactOptimal 10.1 www.factsage.com Example 7 : Target Optimization - 2 We are searching for compositions for which the density of the liquid at the liquidus temperature is 2.00 g/ml. Note: if you click here. the logarithm of the objective function will be optimized. This may present a numerical advantage, increasing the speed and precision of the calculation in some cases The value of Delta is the normalized interval of precision. Any solution within this range of tolerance will be accepted by FactOptimal. In this example we choose an error of 2.5%. FactOptimal 10.2 www.factsage.com Example 7 : Target Optimization - 3 Here FactOptimal minimizes the error between the current calculated density and the targeted density. The best solution is displayed in the table at the end of the optimization. Click on a line in the spreadsheet and then on « Open in Equilib » to load this calculation in Equilib. The graph shows the error value versus the number of calculations. FactOptimal 10.3 www.factsage.com Example 7 : Target Optimization - 4 The user can click on Continue Run >> to perform another 50 calculations and get a different point targeting the same density. FactOptimal 10.4 www.factsage.com Optimization using the Function Builder - 1 In addition to optimizing properties that can be calculated by Equilib, FactOptimal also allows optimization of user-defined properties, in the form of functions of properties calculated by Equilib. For example, Redkin [1] has proposed that the electrical conductivity σ of molten chloride solutions can be expressed as : ln(σ) = 4.9*exp[-(2747-33724/V)/T]*exp(53.7/V) where V is the volume of the solution in litres. This formula can be saved in the Function Builder and then chosen as a property to be optimized. For examples of the use of Function Builder, see the Function Builder Slide Show. [1] A. Redkin, Relationship between Electrical Conductivity and Thermodynamic Properties of Binary Molten Salt Mixtures http://www.electrochem.org/dl/ma/201/pdfs/1420.pdf FactOptimal 11.1 www.factsage.com Optimization using the Function Builder - 2 Click on the Function Builder icon to open the FactSage Function Builder. Edit or build a new group of functions, then save it. For help click on the Function Builder icon and then on ‘Help > SlideShow’ FactOptimal 11.2 www.factsage.com Optimization using the Function Builder - 3 Here we enter the formula for electrical conductivity in the Function Builder. A group of functions is created in Function Builder, saved as « Electrical Conductivity ln(x) ». We want to use the fuction f1 from this group (a group can contain up to 10 functions f1, f2, f3, etc.) To minimize the Electrical Conductivity, select the saved function as the first property. FactOptimal 11.3 www.factsage.com Optimization using the Function Builder - 4 In this example, the temperature is set as an additional variable. FactOptimal will now determine the composition and temperature which minimize the electrical conductivity. FactOptimal 11.4 www.factsage.com Optimization using the Function Builder - 4 Additional options can then be selected and the Electrical Conductivity can be optimized. FactOptimal 11.5 www.factsage.com Characteristic points on the liquidus surface www.factsage.com What is a characteristic point on the liquidus surface Eutectics, peritectics, monotectics, quasi-peritectics, minima and congruent melting points are characteristic points on the liquidus surface. FactOptimal is able to calculate the compositions of eutectics, minima and congruent melting points. For example, within the Al2O3-ZnO system there is 1 eutectic (E), 1 minimum (MIN), 1 peritectic and 3 congruent melting points (CM). CM P CM CM MIN E We can calculate all these points with FactOptimal except for the peritectic. Clearly, for a binary system it is not necessary to use FactOptimal since the characteristic points are all given by the Phase Diagram module (or can be calculated with a Target option in the Equilib module). We use a binary example here simply to illustrate the input to FactOptimal. FactOptimal 12.1 www.factsage.com Example 8 : How to calculate characteristic points with FactOptimal for the Al2O3-ZnO system -1 Step 1: define the system, select appropriate databases (in this case FTOxid), select a formation target (F) on the liquidus and perform a single calculation at an arbitrary composition. FactOptimal 12.2 www.factsage.com Example 8 : How to calculate characteristic points with FactOptimal for the Al2O3-ZnO system - 2 Step 2: Click on the FactOptimal icon, select “characteristic points on liquidus surface” and start the calculation. If you are using the stored example files, click on “Recent...” to load the FactOptimal file. Precision parameters. The normal precision is recommended for multicomponent systems (N>4) in order to reduce computation time. For multicomponent systems the calculation of the characteristic points on the liquidus surface is usually lengthy . If the calculation should fail unexpectedly, the user can restart the calculation from the results of the previous calculation FactOptimal 12.3 www.factsage.com Example 8 : How to calculate characteristic points with FactOptimal for the Al2O3-ZnO system - 3 FactOptimal Results Window : composition of the 5 characteristic points (MIN, E and CM) for Al2O3-ZnO, as well as the liquidus temperature and enthalpy of melting at each point. FactOptimal keeps searching for points until the user clicks on the Stop button. Click on a point on the graph and then on “Open in Equilib” in order to see the output for that point FactOptimal 12.4 www.factsage.com And for higher order systems ? Of course, for systems of 2 and 3 components, all the characteristic points can also be obtained with the Phase Diagram module: for binary systems a simple (T,X) calculation, and for ternary systems a liquidus projection. Peritectics FactOptimal 12.5 www.factsage.com Characteristic points on the CaO-Al2O3-MgO-SiO2 liquidus Applying the same procedure as previously one can calculate the characteristic points on the liquidus surface of the CaO-Al2O3-MgO-SiO2 system. By clicking on any point on the graph, you can obtain compositions of the characteristic points, the liquidus temperatures and the enthalpies of melting. MgO CaO SiO2 Al2O3 3098 2845 2639 2327 2260 2195 1996 1877 1867 1821 1820 1802 1710 1665 1647 1642 1640 1639 1636 1635 1605 1604 1582 1566 1531 1.0 1519 1436 1.1 0.9 0.8 mol. fract. 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 # Special point Tliquidus The points can be saved as a text file and opened in Excel for post treatment The solid phases that precipitate at the minimum can be seen by opening Equilib FactOptimal 12.6 www.factsage.com Characteristic points on the Al-Mg-Ce-Mn-Y-Zn liquidus Sometimes for large systems when many phases are involved, the calculations can be very time consuming. The user can stop (1) the calculations at any time. However the calculation can be restarted later without losing the previous results (2). The absolute minimum liquidus temperature will always be calculated relatively early in the calculation. 1 In this example, we stopped the calculations after calculating the absolute minimum liquidus temperature and 70 other characteristic points. 2 FactOptimal 12.7 www.factsage.com Characteristic points – reciprocal systems In this example, we wish to calculate characteristic points on the liquidus of a reciprocal salt system (a system with 2 or more cations and 2 or more anions) : Li+, Na+, K+, Mg++, Ca++ / F-, Cl-. WRONG ! Make sure that the input components include all pairs of cations and anions (i.e. all possible end-members). Here we are missing two components : CaF2 and MgF2. FactOptimal 13.1 www.factsage.com Characteristic points – reciprocal systems The correct input contains every end-member (cation-anion pair) in the liquid phase. CORRECT ! FactOptimal 13.2 www.factsage.com Characteristic points – reciprocal systems We choose the Characteristic points on liquidus surface option with the default settings. FactOptimal 13.3 www.factsage.com Characteristic points – reciprocal systems Calculated Characteristic Points in the Li+, Na+, K+, Mg++, Ca++ / F-, Cl- reciprocal system. Right-click anywhere in the table to see this menu, allowing you to save an Excel file. FactOptimal 13.4 www.factsage.com Closest Characteristic point (to initial composition) on the liquidus surface www.factsage.com Example 9: Characteristic points – closest characteristic point - 1 In this example, we wish to calculate the Characteristic point closest to the initial composition Use Default selection option and formation target on the liquid Select the FTsalt database Define the initial composition in Equilib FactOptimal 14.1 www.factsage.com Example 9: Characteristic points – closest characteristic point - 2 Calculate in Equilib and click on the FactOptmal icon in the Results window. Select Characteristic points on liquidus surface and the closest to initial point option Keep default values and click “calculate” The composition, liquidus temperature, heat of melting and the number of solid phases precipitating at the minimum are given in the table. FactOptimal 14.2 www.factsage.com Example 9: Characteristic points – closest Characteristic point - 3 Once the optimization is complete, Equilib will automatically load the calculated point. 0.45484 LiF + 0.13427 NaF + 0.40221 KF + 0.40065 mol AlkF(ssA)#1 (23.173 gram, 0.40065 mol) (728.71 K, 1 bar, a=1.0000) ( 1.6027E-02 NaF + 0.98397 KF) + 0.13376 mol NaF-[LiF](ss) (5.5216 gram, 0.13376 mol) (728.71 K, 1 bar, a=1.0000) ( 4.4221E-02 LiF + 0.95578 NaF) + 8.68E-03 mol CAMX3-Perovskite#1 (1.1595 gram, 8.6800E-03 mol) (728.71 K, 1 bar, a=1.0000) ( 8.0648E-02 LiCaF3 + 4.1687E-10 NaCaF3 + 0.91935 KCaF3) 0 8.680000E-03 CaF2 = In this example, the closest local minimum found by FactOptimal is a Eutectic since 4 phases are in equilibrium with the liquid. FactOptimal found the closest local minimum on the liquidus surface of the quaternary system without trying to find a closer one in subsystems. mol ASalt-liquid#1 (728.71 K, 1 bar, a=1.0000) ( 0.45484 LiF + 0.13427 NaF + 0.40221 KF + 8.6816E-03 CaF2) + 0.44822 mol LiF_Griceite_(NaCl_rock_salt_structure) (11.627 gram, 0.44822 mol) (728.71 K, 1 bar, S1, a=1.0000) FactOptimal 14.3 www.factsage.com Advanced Examples www.factsage.com Simultaneous optimization of two masses of precipitate under constraints on composition, phases amount and density, with temperature as an optimized variable. Improve the mechanical and corrosion properties of AZ91 by addition of Calcium and Rare Earth elements after a full anneal at 200oC<T<400oC www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 1 We consider an AZ91 base alloy (Mg-Al-Zn). We want to improve the mechanical properties by addition of Rare Earth elements (Ce,La) and calcium by simultaneously: •maximizing the amount of C15-Al2Ca+aAl11Re3 – Al2Ca can improve the tensile and elongation properties of AZ91 due to grain refinement. The formation of thermally stable Al11RE3 fine needle-shaped particles along the grain boundaries significantly improves the creep properties and •maximizing the amount of gAl12Mg17 in order to conserve AZ91 microstructure properties Other constraints employed in this example: •Wt. %(Ce)+Wt. % (La) < 1 (to keep the price reasonable) •density > 1.75 g/cm3 •Wt. %(HCP phase)>90 •the HCP phase must be a single phase (i.e. no miscibility gap) FactOptimal 15.1 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 2 System: AZ91+RE+Ca Step 1: Using Equilib we define the system and select the appropriate database: FTlite and perform a single Equilb calculation. Select only FTlite database The temperature will be chosen as a variable, therefore it is irrelevant in the first Equilib calculation. FactOptimal 15.2 Include molar volumes in order to calculate the density www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 3 Step 2: after a single Equilibrium calculation, open FactOptimal and set up the objectives. The two objectives are the maximum of the mass of two different phases FactOptimal 15.3 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 4 Step 2: after a single Equilibrium calculation, open FactOptimal and set up the objectives. The second objective is a sum of the mass of two precipitates + Note: this is a selected species within a solution FactOptimal 15.4 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 5 Step 3: Set up the range of compositions and temperature. In the variables section, define range of compositions and temperature. The range of composition corresponds to approximately the composition of AZ91 alloys. FactOptimal 15.5 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 6 Step 4: Set up the composition constraints. In the constraints section we click on Composition constraints and select a sum of 100 for all composition variables, and we specify that wt.% La + wt.% Ce ≤1 FactOptimal 15.6 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 7 Step 5: Set up the properties constraints. We select only HCP A3#1 so that HCP is a single phase (no miscibility gap possible) FactOptimal 15.7 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 8 Step 6: Set up the parameters and calculate. The region between the two dashed line, is the region with an acceptable amount of gAl12Mg17 to conserve the typical microstructure of AZ91. Beyond this range the microstructure can be very different. The user has to choose a compositions within this range. FactOptimal 15.8 www.factsage.com Example 10: Improve the mechanical properties of AZ91 by addition of Ca and RE - 9 Step 7: Open a chosen point in Equilib and get the detailed results. Summary of the Equilib file of the selected point on the Optimal Pareto 6.628 Al + 2.058 Zn + 0.22 Ce + 0.343 La + 1.691 Ca + 89.06 Mg = 90.608 gram HCP_A3#1 (90.608 gram, 3.6754 mol, 5.1554E-02 litre, 1.7575 gram/cm3) + 4.3164 gram Gamma_Al12Mg17 (4.3164 gram, 2.7838E-03 mol, 2.0370E-03 litre, 2.1190 gram/cm3) + 4.0502 gram Laves_C15#1 (4.0502 gram, 4.3327E-02 mol, 1.9712E-03 litre, 2.0547 gram/cm3) + 0.95463 gram alpha-Al11RE3 (0.95463 gram, 1.3353E-03 mol, 2.3446E-04 litre, 4.0715 gram/cm3)+ + 7.0761E-02 gram Phi (7.0761E-02 gram, 1.9126E-04 mol, 2.5986E-05 litre, 2.7231 gram/cm3) ***************************************************************** H G V S Cp (J) (J) (litre) (J/K) (J/K) ***************************************************************** 1.36182E+04 -7.25584E+04 5.58228E-02 1.82134E+02 1.21185E+02 Total mass/gram = 100.00 System density/gram/cm3 = 1.7913 FactOptimal 15.9 www.factsage.com Maximizing the total mass of all precipitates after Scheil-Guliver cooling and subsequent full annealing with the temperature as an optimized variable Improvement of the mechanical properties of 7178 aluminum alloy 200<T<500ºC www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 1 We consider 7178 aluminum (Al-Cu-Mn-Mg-Zn-Si). The goal of this example is: •To improve the mechanical properties by maximizing the mass of Al2CuMg precipitate in the FCC matrix after a subsequent full annealing. The annealing temperature is to be optimized in order to maximize the amount of precipitate in the FCC matrix. There are constraints only on the ranges of composition and annealing temperature. FactOptimal 16.1 www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 2 System: 7178 aluminum alloy Step 1: Using Equilib we define the system and select the appropriate database: FTlite. Select only the FTlite database Use a cooling step of 10oC from 1300 to 0ºC FactOptimal 16.2 Select the Cooling calculation L-Option and choose a Scheil-Gulliver cooling calculation www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 3 Step 2: after performing a single Cooling type calculation, open FactOptimal and select the Annealing option. In the present example, the temperature is an optimized variable. The temperature specified here will be the initial temperature. Select the primary phase among the other possible phases. Note that you can select one or more phases in order to recycle the sum of masses of the chosen phases. FactOptimal 16.3 www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 4 Step 3: After saving the primary phase (FCC in the present example), set up the objective. Here we choose only one property to be optimized: maximize the mass of the precipitate Al2CuMg after a subsequent annealing. FactOptimal 16.4 www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 5 Step 4: Set up the ranges of composition and annealing temperature. The range of composition corresponds to approximately the composition of 7178 aluminum alloy Note that wt. % of Si is fixed to be 0.4. FactOptimal 16.5 www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 6 Step 5: Set up the composition constraints. In this example there is only one composition constraint, i.e S wt.%=100 FactOptimal 16.6 www.factsage.com Example 11: Improvement of the mechanical properties of 7178 aluminum alloy - 7 Step 6: Set up the parameters (50 calculations with a large initial search region and a precision of 3) and calculate. Equilib output 24.391 gram FCC_A1#1 (24.391 gram, 0.90078 mol, 9.1659E-03 litre, 2.6611 gram/cm3) + 0.39166 gram Laves_C14#1 (0.39166 gram, 2.6894E-03 mol, 1.5615E-04 litre, 2.5083 gram/cm3) + 1.2993 gram Al12Mn_cubic (1.2993 gram, 3.4309E-03 mol, 4.4253E-04 litre, 2.9362 gram/cm3) + 0.22307 gram Al2CuMg_S-Phase_D172h_-_Cmcm (0.22307 gram, 1.5730E-03 mol, 6.2433E-05 litre, 3.5730 gram/cm3) + 2.4541E-02 gram Mg2Si_cF12-Fm(3)m (2.4541E-02 gram, 3.1999E-04 mol, 1.2444E-05 litre, 1.9721 gram/cm3) NOTE: The value found by Fact Optimal corresponds to the amount of Al2CuMg per mole of reactants. FactOptimal 16.7 www.factsage.com Maximizing the elemental solubility in a given phase under constraints of composition and amounts of phases. Improvement of the texture and grain refinement by maximizing the (molar) solubility of Rare Earths in a Mg matrix at T= 300 oC www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 1 We consider a magnesium system with RE (Ce,La, Nd, Pr, Sm) additives. The goal is to MAXIMIZE the solubility for a single HCP phase in order to improve the texture and the grain refinement properties. OTHER CONSTRAINTS considered in this example : •wt.%(Ce)+ wt.%(La) + wt.%(Nd) + wt.%(Pr) + wt.%(Sm) < 0.2 (in order to keep the cost of raw material reasonable) •%(HCP phase) = 100 (that is, no other phases) •We want a single HCP phase (i.e. no miscibility gap) FactOptimal 17.1 www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 2 Step 1: Set up the system in Equilib. Select the FTlite database only FactOptimal 17.2 www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 3 Step 1: Set up the system in Equilib. In the menu window, click on parameters and select output in mol, since the objective is to maximize the molar solubility Set the temperature to 300oC FactOptimal 17.3 www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 4 Step 2: after performing a single calculation, open FactOptimal and set up the problem. To maximize the molar solubility of RE elements in HCP matrix, select all the RE elements in HCP_A3#1 solution without selecting those in HCP_A3#2 since we want a single HCP phase FactOptimal 17.4 www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 5 Step 3: Set up the ranges of composition and constraints. The range of composition depends on the cost of each RE element. S Xi =100 S RE < 0.2 The system must consist of a single HCP phase FactOptimal 17.5 www.factsage.com Example 12: Improve the texture and grain refinement properties at low temperature - 6 Step 4: Set up the parameters (300 calculations with a large initial search region and a precision of 5) and calculate. The Equilib file corresponding to the optimal value of the solubility is automatically given at the end of the calculation: FactOptimal 17.6 www.factsage.com Optimize two linked properties The properties are « linked » because the second calculation requires the calculation of the liquidus temperature. Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus www.factsage.com Example 13: Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus - 1 For the oxide system defined below, we want to minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus Step 1: Set up the system, select the database and perform a single Equilib calculation Select only the FToxid database Select P option on the liquid in order to calculate the liquidus temperature FactOptimal 18.1 www.factsage.com Example 13: Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus - 2 Step 2: Perform a calculation and open FactOptimal. Then select two linked properties since the second temperature = (TLiquidus-200oC). We consider two properties: 1. We minimize the liquidus temperature 2. We maximize the mass of FToxid*SLAG-liq#1 and FToxid*SLAG-liq#2 Click on the Linked button to set T2 = T1-200oC NOTE: We want to minimize the mass of solids therefore we choose to maximize the mass of liquid. FactOptimal 18.2 www.factsage.com Example 13: Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus - 3 Step 3: Define the range of compositions of each end-member. In this example we work with integer variables and a sum of 1000 in order to fix the precision to be exactly 1e-3. FactOptimal 18.3 www.factsage.com Example 13: Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus - 4 Step 4: define the two constraints (1 and 2) upon the compositions. S Compositions variables =1000 We make sure that SiO2 is the dominant species: SiO2 ≥ (MgO+Al2O3+CaO+PbO+ZnO) FactOptimal 18.4 www.factsage.com Example 13: Minimize the liquidus temperature and minimize the solid fraction 200 oC below the liquidus - 5 Step 5: Set up the parameters (1000 Equilib calculations, with small initial mesh region) and calculate. Click on a point in the Pareto front, and click on Open in Equilib to calculate the phases which are in equilibrium at Tliq-200 oC (gram) 100 MgO + (gram) 75 ZnO + 126 Al2O3 + 50 CaO + 147 PbO + 502 SiO2 = 564.44 gram ASlag-liq#1 (564.44 gram, 7.1058 mol) + 185.66 gram AProtopyroxene (185.66 gram, 0.92357 mol) + 45.921 gram Willemite (45.921 gram, 0.22532 mol) + 129.24 gram Mg2Al4Si5O18_Cordierite (129.24 gram, 0.22094 mol) (1064.83 C, 1 bar, S1, a=1.0000) + 59.447 gram CaAl2Si2O8_Anorthite (59.447 gram, 0.21368 mol) (1064.83 C, 1 bar, S2, a=1.0000) + 15.298 gram SiO2_Tridymite(h) (15.298 gram, 0.25461 mol) (1064.83 C, 1 bar, S4, a=1.0000) FactOptimal 18.5 www.factsage.com Example of double target optimization Target simultaneously a liquidus temperature of 1500ºC and a solid fraction of 0.5 at 100ºC below the liquidus www.factsage.com Example 14: Double target optimization - 1 Set up the system: Al2O3-CaO-SiO2-MgO Select only the FToxid database. Select P option on the liquid FactOptimal 19.1 www.factsage.com Example 14: Double target optimization - 2 Setup the problem The first target is a liquidus temperature of 1500 oC +/- 1% • The two properties are linked: click on the linked button and specify the second temperature to be 100 oC below the liquidus • We target the solid fraction to be 0.5. This is equivalent to targeting the liquid fraction to be 0.5. • We need to select both Slag-Liq#1 and Slag-Liq#2 since there is a possible miscibility gap The second target is a liquid mass fraction 100 oC below the liquidus of 0.5 +/- 1% FactOptimal 19.2 www.factsage.com Example 14: Double target optimization - 3 There are no constraints, except Sxi=1, setup 250 calculations with an initial mesh size of 1 and a precision of 3 then calculate. The results show a Pareto front which minimizes simultaneously the error on both targets. The user then has to choose the better compromise according his own requirements. Open in Equilb and get the solids phases which precipitate at 100 oC below the liquidus 0.593 Al2O3 + 0.03 MgO = 0.376 CaO + 0.001 SiO2 + 0.54805 gram ASlag-liq#1 (0.54805 gram, 7.5624E-03 mol) + 0.45195 gram CaAl2O4_solid (0.45195 gram, 2.8597E-03 mol) This composition is potentially the best one FactOptimal 19.3 www.factsage.com Example 14: Double target optimization - 4 We ran the optimization for 2000 calculations. Fact Optimal stopped after 1558 calculations and found a solution with a very small error on both objectives. 0.49275 gram ASlag-liq#1 (0.49275 gram, 7.0244E-03 mol) + 0.43700 gram Melilite (0.43700 gram, 1.5940E-03 mol) + 4.3242E-02 gram a-Ca2SiO4 (4.3242E-02 gram, 2.5248E-04 mol) + 2.7011E-02 gram CaAl2O4_solid (2.7011E-02 gram, 1.7092E-04 mol) FactOptimal 19.4 www.factsage.com Example 14: Double target optimization - 5 For a difficult system or a system where the best starting point is unknown, using Quasi-Random calculations could actually provide better results than running a high number of optimization calculations. Here we did 500 Quasi-Random calculations and 500 optimization calculations and obtained a slightly better solution than in the previous slide. We get almost the ideal solution: 0.49712 gram ASlag-liq#1 + 0.37811 gram a'Ca2SiO4 + 0.11655 gram Aspinel + 8.2194E-03 gram FactOptimal 19.5 AMonoxide#1 www.factsage.com

Download
# The FactOptimal module